Research Letter | Open Access
D. P. Das, K. M. Parida, B. K. Mishra, "Synthesis and Surface Properties of Silica Spheres with Core Shell Structure by One Convenient Method", Advances in Materials Science and Engineering, vol. 2009, Article ID 328508, 5 pages, 2009. https://doi.org/10.1155/2009/328508
Synthesis and Surface Properties of Silica Spheres with Core Shell Structure by One Convenient Method
Earlier, we have published a paper on the preparation of silica sphere using propanol as cosurfactant. We report here a highly cost-effective method of preparation of mesoporous silica spheres with core shell structure using sodium silicate as silica precursor, cetyltrimethyl ammonium bromide (CTAB) as surfactant, and methanol as cosurfactant. Thus after removal of the template by dissolutions or/and activation at higher temperature, mesoporous silica spheres with core shell structure were obtained. The products prepared with methanol to CTAB molar ratio 8.5 : 1 were confirmed to give best results. All the spherical products have very large surface area (589–1044 /g), pore volume (0.98–1.41 c/g), and ordered pore structure.
The synthesis of ordered mesoporous metal oxide using surfactant templating was first reported by Kresge et al. and Beck et al. in 1992 [1, 2]. Since then, ordered mesoporous metal oxides have been the topic of rapid discovery in material chemistry, catalysis, chemical sensing, and separations [3, 4]. Silica spheres have almost been obtained by using a biphasic system of a quaternary ammonium surfactant [5–7], that recently has been synthesized using the nonionic polyethylene-oxide-based surfactant by Boissiére et al.  and dual templates by Yang et al. . Silica spheres of hollow morphologies have attracted much attention due to their potential applications in drug-delivery, adsorption, and catalysis . Hollow spheres may also provide some immediate advantages over their solid counter parts because of their relatively low densities . Several chemical and physicochemical methods have been used to synthesize hollow spheres, including emulsion phase separation techniques, emulsion interfacial polymerization, and templating colloidal particle techniques . Li et al.  reported the isolation of hollow silica spheres taking calcium carbonate nanoparticles as templating agent and sodium silicate as silica source for drug delivery applications. Very recently, Zhang et al.  prepared hollow monodispersed silica spheres from TEOS by varying water to ethanol molar ratio under sonication environment. Naik and Sokolov  reported the preparation of nanoporous silica spheres at room temperature using sodium metasilicate as silica precursor and CTACl as structure directing agent.
The present work is an extension of our previous work reported elsewhere  to get hollow silica spheres. We report here a cost effective, simple, and convenient method for the preparation of well-ordered hollow mesoporous silica spheres taking CTAB and methanol as templating agents and sodium silicate as silica source. The materials were characterized by small-angle X-ray diffraction (SXRD), adsorption-desorption, pore size distribution, BET-surface area (Brunauer-Emmett-Teller), particle size distribution, scanning electron microscopy (SEM), and high-resolution transmission electron microscopy (HRTEM).
2.1. Material Synthesis
In a typical synthesis, 10.76 mmol of cetyltrimethyl ammonium bromide (CTAB) was dissolved in 50 mL of double distilled water. Methanol was added to the above solution maintaining the molar ratio of methanol to CTAB in the range of to A solution containing 4 g of sodium silicate, was added to the above mixture with constant stirring at room temperature. The total volume of the solution was kept at 140 mL. About 10 mL of ethyl acetate was added to the above solution and was continuously stirred for 5 hours. After complete hydrolysis, the mixture containing the gel was kept in the oven at for 72 hours. The resulting product was recovered by filtration followed by washing with double distilled water and ethanol. The washed particles were kept at and further activated at for 6 hours to get the hollow structure.
2.2. Methods of Characterization
X-ray diffractograms were recorded on a Rigaku Miniflex (set at 30 kV and 15 mA) powder diffractometer using Cu radiation within the range from 1 to at a rate of /min in steps of . Nitrogen sorption isotherms were recorded at liquid nitrogen temperature () on ASAP 2020 (Micromeritics, USA). Prior to analysis, the particles were subjected to vacuum ( torr) at in order to ensure a clean surface. Surface areas were calculated using Brunauer-Emmett-Teller (BET) method. The pore volumes were taken at relative pressure of 0.95. Pore size distributions were analyzed using Barrett-Joyner-Halenda model. Specimens for SEM were prepared by placing the particles on the carbon tape and coated with gold by sputtering. The sample grids were examined by SEM (Hitachi S-3400N). Particle size analysis of all the mesoporous materials was carried out by Nanotrac 150 (Microtrac Instruments) with sodium hexametaphosphate as dispersant. High-resolution transmission electron microscopic (HRTEM) images were obtained on JEOL JEM 2010, in which samples were prepared by dispersing the powdered samples in 2-propanol by sonication for 20 minutes and then drop-drying on a copper grid coated with carbon film.
3. Results and Discussion
3.1. Characterization by Small-Angle XRD, Sorption at 19 and Particle Size Analysis
The SXRD pattern shows three diffraction peaks indexed as , and (Figure 1). This indicates that the pore structure of the mesoporous silica is in a hexagonal array as was reported by Lin and Mou . The interplanar distance and the distance between pore centers, represented by the d-values of diffraction peak and the -values (), respectively, were listed in Table 1. The -values increase with increasing molar ratio of methanol to CTAB. Since the mesoporous silica spheres were synthesized using the micelles as templates, we believe that the size of the micelles increased with increase in the amount of methanol. This is also expected, as methanol could only be solubilized in the palisade layer of the micelles . As a consequence there is an increase in the distance between two adjacent pore centers.
aCalculated from SXRD.|
bCalculated from the desorption portion of N2 adsorption-desorption isotherm.
From Figure 2, all the samples were observed to follow the type IV isotherm, H1 hysteresis loop. From Figures 2 and 2– for molar ratios , and , respectively, clear adsorption steps of capillary condensation were observed indicating the larger mesopore diameter and uniformity of framework mesoporosity. The materials are observed to be of not exactly MCM 41, rather MCM 41 type. The isotherm in Figure 2 for the product obtained with methanol to CTAB ratio exhibits no such clear steps. The result indicates that the pore size of the synthesized silica was found in the range of mesoscale which is in agreement with Sing et al. . Specific surface area and total pore volume were listed in Table 1. All the samples have very high surface area ( m2/g) and pore volume ( cm3/g). The average pore size increases with increase in the methanol to CTAB ratio (Figure 3). From Figure 3, the pore size of all the materials was observed to be unimodal in character. This is in agreement with SXRD. At the same time, total pore volume also increases with increase in the molar ratio of methanol to CTAB (see Table 1). This shows that an optimum amount of methanol is required for the formation of a more ordered pore structure and also helps in increasing the total pore volume. This is in support of particle size analysis (inset of Figure 1).
3.2. SEM and TEM Observations
From Figure 4, the spherical particles with multiple of micrometer size were observed by varying the molar ratio of methanol to CTAB (from to ). Also, it is clearly visible from Figures 4(a), 4(f), and 4(g) that the particles have core shell structure. This structure has been destroyed at molar ratio of (Figure 4(e)). Again, one can clearly notice from Figures 4(h), 4(i), and 4(j) that the particles are still spherical and hollow at 600 for the molar ratio . The wall thickness was found to be nm from TEM micrographs. This is not clearly observed from Figure 4(k) due to the incomplete removal of the template at 540. Again, Figure 4(l) shows the close packed hexagonal structure of mesoporous silica as well as the existence of uniform pores in the wall of hollow silica sphere. As the formation of particles is templated by micelles, the morphology changes with the molar ratio of methanol to CTAB. Above the critical micelle concentration (CMC), the size and the shapes of micelles changed in response to increase in the CTAB concentration. Again, with excess of methanol the shape of the micelles could be transformed to spheres . Ethyl acetate was added to control the solution pH. It is soluble in the palisade layer of the CTAB micelles. Its hydrolysis is catalyzed by cationic micelles to form acetic acid:
The acetic acid formed during hydrolysis may possibly be neutralized by sodium silicate on the CTAB micelle surface. Therefore the pH value of the solution decreased gradually from basic to neutral conditions, and finally silica is formed. Furthermore, the morphology of mesoporous silica is also dependent on the hydrophobic interactions between CTAB and methanol which were self-assembled onto mesoporous silica. It has been observed by Zana  that with increase in methanol concentration (above molar ratio) the hydrophobic interactions between the molecules of adsorbed methanol and CTAB on the surface of colloidal seeds get weakened. For this reason we believe that the pore structure of the resulting silica spheres became less ordered. However, correlating our previous work  with present investigation, a question might be raised why propanol/CTAB system gives solid spheres whereas methanol/CTAB system gives core shell structures? Previous investigations have shown that the self-assembly of organic-inorganic hybrid system can be explained in terms of surfactant packing parameter/critical aggregation parameter, (()) , where “” is the total volume of the surfactant chain plus any cosolvent molecules between the chains, “” is the effective head group area at the organic-inorganic interface and “” is the surfactant chain length. Depending on the cosolvent or swelling agent chain length, the “” will vary and consequently “”. Hence, we change the -3 to -1, which causes a transformation from solid to core shell structure.
The synthesized silica particles with methanol : CTAB molar ratio below show core shell structure which was evidenced from SEM and TEM micrographs. The sizes of the particles were in the range of 1 to 1.7 micron with very large surface area ( m2/g) and pore volume ( cm3/g) and exhibit ordered pore structure. There existed a type IV adsorption isotherm and H1 hysteresis loop according to IUPAC classification. The most probable pore size increased with increase in the molar ratio of methanol to CTAB. This is in agreement with the small-angle X-ray diffraction data. The small angle XRD patterns reveal that the materials are MCM 41 type.
The authors are thankful to Dr. K. S. Rama Rao, IICT, Hyderabad, India for small-angle XRD analyses and Dr. B. Satapati, IMMT, Bhubaneswar for TEM analyses. One of the authors, D. P. Das., is grateful to CSIR, New Delhi, for providing a Research Associateship. Financial assistance by DST, Government. of India, is greatly acknowledged.
- C. T. Kresge, M. E. Leonowicz, W. J. Roth, J. C. Vartuli, and J. S. Beck, “Ordered mesoporous molecular sieves synthesized by a liquid-crystal template mechanism,” Nature, vol. 359, no. 6397, pp. 710–712, 1992.
- J. S. Beck, J. C. Vartuli, W. J. Roth et al., “A new family of mesoporous molecular sieves prepared with liquid crystal templates,” Journal of the American Chemical Society, vol. 114, no. 27, pp. 10834–10843, 1992.
- A. Corma and D. Kumar, “Possibilities of mesoporous materials in catalysis,” in Proceedings of the 1st International Symposium on Mesoporous Molecules Sieves, L. Bonneviot, F. Béland, C. Danumah, S. Giasson, and S. Kaliaguine, Eds., vol. 117 of Studies in Surface Science and Catalysis, pp. 201–222, Baltimore, Md, USA, July 1998.
- X. S. Zhao, G. Q. Lu, and G. J. Millar, “Advances in mesoporous molecular sieve MCM-41,” Industrial and Engineering Chemistry Research, vol. 35, no. 7, pp. 2075–2090, 1996.
- Q. Huo, J. Feng, F. Schüth, and G. D. Stucky, “Preparation of hard mesoporous silica spheres,” Chemistry of Materials, vol. 9, pp. 14–17, 1997.
- H. Yang, G. Vovk, N. Coombs, I. Sokolov, and G. A. Ozin, “Synthesis of mesoporous silica spheres under quiescent aqueous acidic conditions,” Journal of Materials Chemistry, vol. 8, no. 3, pp. 743–750, 1998.
- L. Qi, J. Ma, H. Cheng, and Z. Zhao, “Micrometer-sized mesoporous silica spheres grown under static conditions,” Chemistry of Materials, vol. 10, no. 6, pp. 1623–1626, 1998.
- C. Boissière, A. van der Lee, A. El Mansouri, A. Larbot, and E. Prouzet, “A double step synthesis of mesoporous micrometric spherical MSU-X silica particles,” Chemical Communications, no. 20, pp. 2047–2048, 1999.
- M. Yang, G. Wang, and Z. Yang, “Synthesis of hollow spheres with mesoporous silica nanoparticles shell,” Materials Chemistry and Physics, vol. 111, no. 1, pp. 5–8, 2008.
- J.-H. Park, Y.-G. Kim, C. Oh et al., “Fabrication of hollow silver spheres by MPTMS-functionalized hollow silica spheres as templates,” Materials Research Bulletin, vol. 40, no. 2, pp. 271–280, 2005.
- T. K. Mandal, M. S. Fleming, and D. R. Walt, “Production of hollow polymeric microspheres by surface-confined living radical polymerization on silica templates,” Chemistry of Materials, vol. 12, no. 11, pp. 3481–3487, 2000.
- X. Cheng, S. Liu, L. Lu et al., “Fast fabrication of hollow silica spheres with thermally stable nanoporous shells,” Microporous and Mesoporous Materials, vol. 98, no. 1–3, pp. 41–46, 2007.
- Z.-Z. Li, L.-X. Wen, L. Shao, and J.-F. Chen, “Fabrication of porous hollow silica nanoparticles and their applications in drug release control,” Journal of Controlled Release, vol. 98, no. 2, pp. 245–254, 2004.
- H. Zhang, J. Wu, L. Zhou, D. Zhang, and L. Qi, “Facile synthesis of monodisperse microspheres and gigantic hollow shells of mesoporous silica in mixed water-ethanol solvents,” Langmuir, vol. 23, no. 3, pp. 1107–1113, 2007.
- S. P. Naik and I. Sokolov, “Room temperature synthesis of nanoporous silica spheres and their formation mechanism,” Solid State Communications, vol. 144, no. 10-11, pp. 437–440, 2007.
- D. P. Das, K. M. Parida, and B. K. Mishra, “A study on the structural properties of mesoporous silica spheres,” Materials Letters, vol. 61, no. 18, pp. 3942–3945, 2007.
- H.-P. Lin and C.-Y. Mou, “‘Tubules-within-a-tubule’ hierarchical order of mesoporous molecular sieves in MCM-41,” Science, vol. 273, no. 5276, pp. 765–768, 1996.
- G. Zhao, in Physical Chemistry of Surfactants, chapter 4, p. 184, Beijing University Press, Beijing, China, 1984.
- K. S. W. Sing, D. H. Everett, R. A. W . Haul et al., “Reporting physisorption data for gas/solid systems with special reference to the determination of surface-area and porosity (recommendations 1984),” Pure and Applied Chemistry, vol. 57, no. 4, pp. 603–619, 1985.
- H. Hoffmann, “Fascinating phenomena in surfactant chemistry,” Advanced Materials, vol. 6, no. 2, pp. 116–129, 1994.
- R. Zana, “Aqueous surfactant-alcohol systems: a review,” Advances in Colloid and Interface Science, vol. 57, pp. 1–64, 1995.
- Q. Huo, D. I. Margolese, and G. D. Stucky, “Surfactant control of phases in the synthesis of mesoporous silica-based materials,” Chemistry of Materials, vol. 8, no. 5, pp. 1147–1160, 1996.
Copyright © 2009 D. P. Das et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.